Fabrication of Ln-MOFs with color-tunable photoluminescence and sensing for small molecules
Wang, Shengyan; Shan, Liang; Fan, Yong; Jia, Jia; Xu, Jianing; Wang, Li; Journal of Solid State Chemistry 245 (2017) 132–137; doi:10.1016/j.jssc.2016.10.006

data_1560688
_publ_section_title
;
 Fabrication of Ln-MOFs with color-tunable photoluminescence and sensing
 for small molecules
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              132
_journal_page_last               137
_journal_paper_doi               10.1016/j.jssc.2016.10.006
_journal_volume                  245
_journal_year                    2017
_chemical_formula_sum            'C15 H7 Eu N0 O9'
_chemical_formula_weight         483.17
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                71.49(3)
_cell_angle_beta                 80.36(3)
_cell_angle_gamma                64.27(3)
_cell_formula_units_Z            2
_cell_length_a                   9.2809(19)
_cell_length_b                   9.6946(19)
_cell_length_c                   11.191(2)
_cell_measurement_reflns_used    996
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.02
_cell_measurement_theta_min      3.01
_cell_volume                     859.6(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  RAXIS-RAPID
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0313
_diffrn_reflns_av_sigmaI/netI    0.0429
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            8477
_diffrn_reflns_theta_full        27.46
_diffrn_reflns_theta_max         27.46
_diffrn_reflns_theta_min         3.05
_exptl_absorpt_coefficient_mu    3.692
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.867
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             464
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_refine_diff_density_max         1.031
_refine_diff_density_min         -1.281
_refine_diff_density_rms         0.199
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.104
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     226
_refine_ls_number_reflns         3881
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.104
_refine_ls_R_factor_all          0.0363
_refine_ls_R_factor_gt           0.0316
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0512P)^2^+1.6098P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0879
_refine_ls_wR_factor_ref         0.0895
_reflns_number_gt                3513
_reflns_number_total             3881
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2017-245-132.CIF
_cod_data_source_block           w
_cod_original_cell_volume        859.6(3)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1560688